1. Introduction to Silicone ChemistryA. Colas, Dow Corning Europe SA, Seneffe (Belgium)By analogy with ketones, the name “silicone” was given in 1901 by Kipping to describe newcompounds of the brut formula R2SiO. These were rapidly identified as being polymeric andactually corresponding to polydialkylsiloxanes. Among them, the most common arepolydimethylsiloxanes (PDMS), trimethylsilyloxy terminated with the structure:The methyl groups along the chain can be substituted by many other groups (e.g., phenyl,vinyl or trifluoropropyl). The simultaneous presence of “organic” groups attached to an“inorganic” backbone gives silicones a combination of unique properties and allows their usein fields as different as aerospace (low and high temperature performance), electronics(electrical insulation), health care (excellent biocompatibility) or in the building industries(resistance to weathering).NomenclatureThe main chain unit in PDMS, - (SiMe2O) -, is often shortened to the letter D because, as thesilicon atom is connected with two oxygen atoms, this unit is capable of expanding within thepolymer in two directions. In a similar way, M, T and Q units can be defined correspondingto :The above polymer (1) can also be described as MDnM. This allows simplifying thedescription of various structures like (Me3SiO)4Si or tetrakis(trimethylsilyloxy)silane, whichbecomes M4Q. Superscripts are sometimes used to indicate groups other than methyl (e.g.,DH for HMeSiO2/2).
The synthesis of siloxanes has been described elsewhere [1, 2, 3]. In summary, PDMS isobtained from the hydrolysis of dimethyldichlorosilane Me2SiCl2, which leads to a mixtureof linear and cyclic oligomers:Higher molecular weight PDMS is obtained after polymerisation, for example, of the abovecyclics in the presence of an end-blocker such as hexamethyldisiloxane and catalysed by astrong acid or strong base according to:Using other chlorosilanes, different end-blockers and/or different cyclics leads to manystructures including polymers with various functional groups grafted on the polymer chainand/or at the polymer ends (e.g., vinyl, hydrogeno, phenyl, amino alkyl). These can beformulated into solvent-based, emulsion or solventless products.Reactive polymers can be cross-linked into elastomers using: • a peroxide-initiated reaction; in particular, if the silicone polymer carries some vinyl groups • a condensation reaction; for example, between a hydroxy end-blocked PDMS and an alkoxysilane, in presence of tin salt or titanium alkoxide as catalyst • an addition reaction; for example, between a vinyl-functional PDMS and an hydrogenomethyl dimethyl siloxane oligomer, in presence of a organic platinum complexSuch polymer, cross-linker and catalyst are formulated with various additives as one-part,ready-to-use products or two-part products to be mixed prior to use and to cure at roomtemperature or only at elevated temperatures.Physicochemical PropertiesThe position of silicon, just under carbon in the periodic table, led to a belief in the existenceof analogue compounds where silicon would replace carbon. Most of these analoguecompounds do not exist, or if they do, they behave very differently. There are few similaritiesbetween Si-X bonds in silicones and C-X bonds [1-3]: Element (X) Bond length (Å) Ionic character ( %) Si - X C-X Si - X C-X Si 2.34 1.88 -- 12 C 1.88 1.54 12 -- H 1.47 1.07 2 4 O 1.63 1.42 50 22
Between any given element and silicon, bond lengths are longer than for carbon with thiselement. The lower silicon electronegativity (1.8) vs. carbon (2.5) leads to a verypolarised Si-O bond, highly ionic and with a large bond energy, 452 kJ/mole (108 kcal/mol).The Si-C bond has a bond energy of ±318 kJ/mole (76 kcal/mol), slightly lower than a C-Cbond, while the Si-Si bond is weak, 193 kJ/mole (46.4 kcal/mole). These values partiallyexplain the stability of silicones; the Si-O bond is highly resistant to homolytic scission. Onthe other hand, heterolytic scissions are easy, as demonstrated by the re-equilibrationreactions occurring during polymerisations catalysed by acids or bases. Silicon atoms do notform stable double or triple bonds of the type sp2 or sp with other elements, yet the proximityof the d orbitals allows d -p retro-coordination. Because of this retro-coordination,trialkylsilanols are more acid than the corresponding alcohols. Yet, the involvement of retro-coordination is challenged .Another example of the difference between analogues is the tetravalent diphenyldisilanol,(C6H5)2Si(OH)2, which is stable, while its carbon equivalent, a gem-diol, dehydrates. The Si-H bond is weakly polarised, but here in the direction of a hydride, and is more reactive thanthe C-H bond. Overall, there are few similarities between a silicone polymer and ahydrocarbon polymer.Silicones display the unusual combination of an inorganic chain similar to silicates and oftenassociated with high surface energy but with side methyl groups that are, on the contrary,very organic and often associated with low surface energy . The Si-O bond are stronglypolarised and without protection should lead to strong intermolecular interactions. However,the methyl groups, only weakly interacting with each other, shield the main chain.This is made easier by the high flexibility of the siloxane chain; rotation barriers are low, andthe siloxane chain can adopt many conformations. Rotation energy around a CH2-CH2 bond in polyethylene is 13.8 kJ/mol but only 3.3 kJ/mol around a Me2Si-O bond,corresponding to a nearly free rotation. The siloxane chain adopts a configuration that can beidealised by saying that the chain exposes a maximum number of methyl groups to theoutside, while in hydrocarbon polymers, the relative backbone rigidity does not allow“selective” exposure of the most organic or hydrophobic methyl groups. Chain-to-chaininteractions are low, and the distance between adjacent chains is also higher in silicones.Despite a very polar chain, silicones can be compared to paraffin, with a low critical surfacetension of wetting . Yet because of their low intermolecular forces, PDMS materialsremain liquid in a much wider range of molecular weights and viscosities than hydrocarbons.The surface activity of silicones is displayed in many circumstances : • Polydimethylsiloxanes have a low surface tension (20.4 mN/m) and are capable of wetting most surfaces. With the methyl groups pointing to the outside, this gives very hydrophobic films and a surface with good release properties, particularly if the film is cured after application. Silicone surface tension is also in the most promising range considered for biocompatible elastomers (20 to 30 mN/m). • Silicones have a critical surface tension of wetting (24 mN/m), which is higher than their own surface tension. This means that silicones are capable of wetting themselves, a property that promotes good film formation and good surface covering. • Silicone organic copolymers can be prepared with surfactant properties, with the silicone as the hydrophobic part (e.g., in silicone polyether copolymers).
The low intermolecular interactions in silicones have other consequences : • Glass transition temperatures are very low (e.g., 146 K for a polydimethylsiloxane compared to 200 K for polyisobutylene, the analogue hydrocarbon); cross-linked PDMS will be elastomeric at RT in the absence of any plasticizers. • The presence of a high free volume compared to hydrocarbons explains the high solubility and high diffusion coefficient of gas into silicones. Silicones have a high permeability to oxygen, nitrogen and water vapour, even if in this case liquid water is not capable of wetting a silicone surface. As expected, silicone compressibility is also high. • In silicone, the activation energy to the viscous movement is very low, and viscosity is less dependent on temperature compared to hydrocarbon polymers. Moreover, chain entanglements are involved at higher temperature and contribute to limit the viscosity reduction .The presence of groups other than methyl along the chain allows modification of some of theabove properties: • A small percentage of phenyl groups along the chain perturbs sufficiently to reduce crystallisation and allows the polymer to remain flexible at very low temperatures. The phenyl groups also increase the refractive index. • Trifluoropropyl groups along the chain change the solubility parameter of the polymer from 7.5 to 9.5 (cal/cm3)1/2. These copolymers are used to prepare elastomers with little swelling in alkane or aromatic solvents.Considering the above, many polymeric “architectures” can be prepared of different physicalforms (volatile, liquid, viscoelastic, solid) with different functionalities, inert or capable ofinteracting or reacting with many other compounds. Formulation into convenient productsleads to even more products. This explains the wide range of industries where silicones areused.
References1 Hardman, B. Encycl. Polym. Sci. Eng. 1989, 15, 204.2 Rochow, E. G. Silicon and Silicones, Springer-Verlag: Berlin, Heidelberg, New York, 1987.3 Noll, W. Chemistry and Technology of Silicones; Academic Press: New York, 1968.4 Owen, M. J. Chemtech. 1981 11, 288. This article has been updated and republished in Chimie Nouvelle 2004, 85, 27.This article has been published in the chapter “Silicones in Industrial Applications” in Inorganic Polymers,an advanced research book by Nova Science Publishers (www.novapublishers.com); edited by Roger DeJaeger (Lab. de Spechtrochimie Infrarouge et Raman, Univ. des Sciences and Tecn. de Lille, France) andMario Gleria (Inst. di Scienze e Tecn. Molecolari, Univ. di Padoa, Italy). Reproduced here with thepermission of the publisher.